HAL Id: hal-02974725
Submitted on 25 Nov 2020
HAL is a multi-disciplinary open access archive for the deposit and dissemination of sci- entific research documents, whether they are pub- lished or not. The documents may come from teaching and research institutions in France or abroad, or from public or private research centers.
L’archive ouverte pluridisciplinaire HAL, est destinée au dépôt et à la diffusion de documents scientifiques de niveau recherche, publiés ou non, émanant des établissements d’enseignement et de recherche français ou étrangers, des laboratoires publics ou privés.
Electrochemical sensors based on molecularly imprinted chitosan: A review
Fares Zouaoui, Saliha Bourouina-Bacha, Mustapha Bourouina, Nicole Jaffrezic-Renault, Nadia Zine, Abdelhamid Errachid
To cite this version:
Fares Zouaoui, Saliha Bourouina-Bacha, Mustapha Bourouina, Nicole Jaffrezic-Renault, Nadia Zine, et
al.. Electrochemical sensors based on molecularly imprinted chitosan: A review. Trends in Analytical
Chemistry, Elsevier, 2020, 130, pp.115982. �10.1016/j.trac.2020.115982�. �hal-02974725�
Electrochemical sensors based on molecularly imprinted chitosan: A review 2
Fares ZOUAOUI1,2, Saliha BOUROUINA-BACHA2, Mustapha BOUROUINA2, Nicole JAFFREZIC-RENAULT1*, Nadia ZINE1,
1 University of Lyon, Institute of Analytical Sciences, UMR 5280, CNRS, 69100 Villeurbanne, France.
2 University of Bejaia, Laboratory of Environmental Engineering, Bejaia, Algeria.
Corresponding authors’ email address:Nicole JAFFREZIC-RENAULT firstname.lastname@example.org
Abdelhamid ERRACHID email@example.com
Despite the enormous development of instruments for analyzing a wide variety of compounds, applied in different fields such as
health, environment or quality control, the demand for increasingly sensitive and selective techniques continues to grow. In this
regard, efforts have been made to highlight more appropriate techniques. Electrochemical sensors based on molecularly imprinted
polymers (MIPs) offer an interesting alternative since they allow reaching high sensitivity and selectivity and they are inexpensive
and easily adaptable to miniaturization. The choice of the functional monomer in the synthesis of MIPs is based on its capacity to
provide complementary interactions with the target molecules. The various excellent properties of chitosan, as a biosourced polymer,
make it a promising alternative to conventional functional monomers. This review reports on the principle of the MIPs technique
describing the different possible approaches in their synthesis. It aims to provide an overview of the value of using chitosan as a
functional monomer by highlighting its applications in electrochemical sensors.
Keywords: Molecularly imprinted polymers, Chitosan, Electrochemical sensors, Electrodepostion, Coating.
Conventional analytical techniques (chromatography, Nuclear Magnetic Resonance (NMR), mass spectrometry (MS), etc.) used for
monitoring in different fields such as medicine, clinical biology, the food industry and the quality control of our environment (monitoring
industrial or domestic discharges) are generally complex, expensive, bulky and often difficult and time-consuming to implement, and
they require highly qualified personnel. In addition, conventional procedures consist in taking samples from the monitored
environments and analyzing them in the laboratory. The steps of sample preparation, incubation, and processing of results often
greatly increase the total analysis time . In order to carry out these analyses, there is a need to set up rapid, simple, inexpensive,
selective techniques and to design compact monitoring tools operating on site, in real time.
Among the devices capable of responding to this demand, sensors present the essential function of detection or even quantification
of a physical, biological or even of a chemical phenomenon in a measurable signal and directly usable by humans. Electrochemical
sensors are a promising choice because of their simplicity, sensitivity, ease of implementation and generally low measurement costs,
but also for their varied applications in the field of health, of the environment or of quality control of food products. Electrochemical
sensors are based on different electrochemical techniques: potentiometry, voltammetry, amperometry, impedimetry .
Biological elements (antibodies, enzymes, microorganisms, DNA, etc.) are generally used for recognition in order to increase
sensitivity and specificity, which are generally lacking in chemical sensors. However, as they are biomolecules, their use is limited to
mild conditions of pH, temperature and nature of the medium in order to avoid denaturating the protein. In addition, using these
biological elements is not so simple. Sourcing them and immobilizing them on the electrode surface require considerable skill [3,4].
Due to the need to overcome these limitations, an alternative has been developed which consists of using molecularly imprinted
polymers (MIPs). MIPs have been used as an artificial recognition material whose binding site size and shape are complementary to
the template molecules for their specific recognition. This approach was established in 1972 by Wulff and Sarhan . To generate
MIPs with selective cavities, a monomer is simply polymerized in the presence of the target molecule and a crosslinking agent leading
to the formation of a highly cross-linked functional monomer/template complex. The formation of the complex has been theoretically
studied in several articles [6,7]. Cavities specific to the target molecule are then obtained after extracting the template from the
polymer. Template/monomer and crosslinking agent/monomer ratios play an important role in the synthesis of MIPs improving the
efficiency [8,9]. MIPs are characterized by very interesting properties such as physical resistance, robustness, resistance to high
pressures and temperatures and high inertia towards various chemicals , and are produced at low cost. In addition, MIPs have a
high affinity and selectivity towards target molecules; they are comparable to natural receptors . MIPs are widely used in various
fields, such as liquid chromatography, capillary electrochromatography, solid phase extraction, therapy, preparation of artificial
antibodies and enzymes, catalysts and syntheses, sensors, etc. [12,13].
The choice of the functional monomer in the synthesis of MIPs is a primordial step given its capacity to provide complementary
interactions with the matrix molecules . Chitosan (CS) is a natural polysaccharide obtained by deacetylation of chitin which is the
most abundant non-toxic, biodegradable and biocompatible natural amino polysaccharide . Chitosan has three types of reactive
functional groups, one amine group and two primary and secondary hydroxyl groups. This structure thus allows numerous chemical
modifications, and can support a succession of chemical reactions such as the reaction with aldehydes and acetones, grafting, H
bond with polar atoms, crosslinking, etc. The functional properties of chitosan films can be improved when combined with other
materials . Due to the positive charges on its amine groups, the cationic biopolymer can interact with anionic molecules. These
unique properties make CS suitable for a wide range of applications in the food, cosmetic and pharmaceutical, sensor and biosensor
fields [17,18]. The presence of reactive functional groups on the polysaccharide chain of CS gives it flexibility, excellent film-forming
capacity, good adhesion, biocompatibility, high mechanical resistance, the possibility of undergoing structural modifications, which
makes it suitable for preparing MIPs and building electrochemical sensors [19,20]. It is well known that the behavior of chitosan can
be affected by several parameters such as pH and humidity [21,22]. Treatment of chitosan with crosslinking agents or by chemical
modification are common strategies to improve its physico-chemical characteristics . Chitosan has been used to make
membranes, thin films and three-dimensional structures. These forms are obtained by different methods such as electrodeposition
 and drop-coating . Electrodeposition is very convenient because it is a simple, fast and low-cost technique, but also it makes
it possible to obtain controlled films .
This review describes the principle of MIPs and the approaches used to synthesize them emphasizing the different criteria for
choosing the reagents and the limitations of this technique. In addition, it accounts for the advantage of using chitosan as a functional
monomer by highlighting its applications in electrochemical sensors.
I. Natural origin of chitosan
I.1. Structure and sources of Chitin
Chitin, first identified in 1884, is the second most abundant biopolymer in nature after cellulose. Its chemical structure consists of N-
acetylglucosamine units. Chitin’s physical structure includes three allomorphs, due to the arrangement of macromolecular chains, α,
β and γ-chitin (figure 1). α-chitin is one of the most abundant allomorphs in which polymer chains are arranged in the same direction
and parallel. β-chitin is less frequent in nature and presents anti-parallel chains. The γ-chitin, according to the studies, is a variant of
the α or β- family .
80 81 82
83 84 85 86 87 88 89
Figure 1: Allomorph types of chitin.
Chitin is present in co-products in the form of chitin-proteins-calcium carbonate complexes . Chitin can be obtained from various
sources (Table 1), it is mainly found in exoskeletons, mollusks and various microorganisms [15,28].
Table 1: Main sources of chitin.
Fungi, yeast cell walls, krill, lobster , crab, tendons, shrimp shells, insect cuticle.
Squid pens, tube synthesized by pogonophoran and vestimentifera worms, lorica built by some seaweeds
I.2. Extraction of chitin
Usually, two types of extraction process are used to obtain pure chitin: chemical and biological methods (Fig.2). Chemical extraction
is based on three stages; between these different stages, washing operations are necessary .
Ø Demineralization: by hydrochloric acid to eliminate minerals. This consists in the elimination of the calcium carbonate and
Ø Deproteinization: by sodium hydroxide to eliminate proteins.
Ø Bleaching: by sodium hypochlorite to remove pigments.
Biological treatments offer an alternative way to extract chitin, to avoid acidic and alkaline treatments. Lactic acid-producing bacteria
and proteases from bacteria have been used for the demineralization and deproteinization steps respectively . Chitin is highly
hydrophobic and insoluble in water and most organic solvents are due to the presence of acetyl groups , so it can be used in
more applications when transformed into chitosan.
I.3. Deacetylation of chitin
The deacetylation step consists in converting chitin to chitosan by the removal of acetyl groups and leads to partial deacetylation.
The border between chitin and chitosan corresponds to a degree of deacetylation (DD). This makes the degree of deacetylation an
important property in the production of chitosan since it determines the free amino groups in the polysaccharides. Indeed, it affects
the physicochemical properties and thus determines its appropriate applications. DD is an important criterion for distinguishing
between chitin and chitosan, defined as the fraction of glucosamine /N-acetyl glucosamine: note that:
Ø for a DD <60%, the polymer is named chitin.
Ø for a DD> 60%, the polymer is named chitosan .
The degree of acetylation controls the proportion of amine and acetyl groups in the carbonic chain and is directly related to the
solubility and acid-base behavior of the polymer . Many methods have been developed to determine DD, such as the
conductimetric assay [32,33], potentiometric titration , UV spectroscopy, IR spectroscopy, 1H NMR spectroscopy, HPLC analysis
, etc. Deacetylation can occur either chemically or enzymatically.
- Chemical deacetylation
Sodium or potassium hydroxides are usually used at high temperature . The alkaline treatment can be repeated to achieve
complete deacetylation . It has been reported that the DD can be affected by temperature, processing time and alkali
concentration. Chemical deacetylation is used more commonly because of its low cost; however, the negative points are high energy
cost, waste of concentrated alkaline solution which leads to an increase in environmental pollution, the fact that it is not easily
controlled and lead to a broad and heterogeneous range of products .
- Enzymatic deacetylation
Chitin deacetylase for the preparation of chitosan polymers is used. It partially catalyses the hydrolysis of N-acetamido bonds in chitin
to produce chitosan [37,38]. Enzymatic deacetylation is a sustainable process and offers the possibility of controlling and predicting
the bioactivities of chitosan. Therefore, the resulting chitosan has a more regular deacetylation pattern than a chitosan treated with
hot alkali [39,40].
Figure 2: Preparation of chitin and chitosan from raw material
II. Properties of chitosan
Chitosan (CS) is the name given to chitin after the deacetylation process (Figure 2). CS is an amino sugar with a molar mass of 179
g/mol glucosamine. It is a family of linear polysaccharides with a molar fraction DD of D-glucosamine and a fraction (1-DD) of N-
acetylglucosamine . Chitosan is thus considered as a copolymer with three types of reactive functional groups, a primary amino
group, and one primary and two secondary hydroxyl groups (one primary amine group (C2) and two hydroxyl groups (C3, C6) per-
repeat unit) (figure 3)
Figure 3: Structure of D-glucosamine
Chitosan is considered as a strongly basic polysaccharide. This polymer has multiple physical and chemical properties that make it
a credible candidate for many applications including foods , pharmaceutical and biomedical , cosmetics, textile and agricultural
, treatment of water and wastewater , etc.
II.2. Molecular weight (Mw), Viscosity and crystallinity of chitosan
Molecular weight (MW) is one of the most fundamental parameters in the characterization of a polymer. Chitosan is a high molecular
weight biopolymer. For a commercial product Mw is 100 to 1200 kilodaltons (kDa); the latter varies according to the sources of raw
materials and the method of preparation. The molecular weight of chitosan is an important characteristic influencing the rheological
properties of the solutions and therefore their conditions of implementation. High molecular weight CS usually gives very viscous
solutions. The determination of Mw can be done by light scattering measurements and viscometry [45,46] or by steric exclusion
Viscosity is one of the most important characteristics of chitosan. The viscosity depends on the DD, Mw and also on the pH value
because these parameters determine the charge density on the polymer chain. The structure of the macromolecules is very extensive
when the charge density is high due to the charge repulsion phenomenon, so viscosity is then hight. On the other hand, when the
polymer is poorly ionized, the macromolecular chains are in the form of statistical balls characterized by low viscosity. As with other
polysaccharides, viscosity drops when the temperature increases .
Crystallinity is also an important parameter because it allows the control of a certain number of properties such as the accessibility
of internal sites in the macromolecular chains, the swelling properties in water or even the diffusional properties. Chitosan is generally
a semi-crystalline material. The crystallinity is usually determined by X-ray diffraction or by NMR .
II.3. Properties of chitosan
Chitosan is a strongly basic polysaccharide, with a cationic character in an acid medium. It is anyway the only water-soluble cationic
polyelectrolyte of natural origin . CS is a hydrophilic biopolymer and a very polar molecule; this property is due to the presence
of numerous hydroxyl and amine groups at the level of the glucosamine units.
It is interesting to note that chitosan is a polycationic polymer having one NH2 group and two OH groups on each glucosamine. These
three groups are very reactive and are very important with respect to the properties of the polymer. The strong functionality of chitosan
gives it a considerable opportunity for chemical modification . The amino groups form a specific binding platform with other
groups external to the polymer, which is an important biofabrication feature . They may cause chemical reactions such as
alkylation, quaternization, reacting with aldehydes and ketones, grafting, etc .
On the other hand, hydroxyl groups give some flexibility to the material and are also responsible for modifying its biological and
physical properties . The hydroxyl functionality also leads to some reactions like o-acetylation, H-bonding with polar atoms, cross-
linking, grafting, etc. .
In contrast to chitin, the presence of free amine groups along the chitosan chain allows this macromolecule to dissolve in diluted
aqueous acidic solvents due to the protonation of these groups, and convert into the ionizable soluble R-NH3+ form [27,51]. This
exceptional peculiarity of being positively charged, allows chitosan to react with negatively charged compounds and to fix them solidly
by ionic bonds, and gives it very numerous properties, such as strong electrostatic interaction, the possibility of hydrogen bonds
formation due to the functional groups and the chain flexibility .
Chitosan can interact with other chemical substances (ions, molecules, macromolecules) thanks to its particular chemical structure
which makes it possible to glimpse capacities to interact, complex or absorb . Chitosan can link functional derivatives on the
macromolecular chains either by covalent, semi-covalent or non-covalent bonds (Figure 4).
Figure 4: Different approaches to complexing chitosan.
At a pH < pKa, the amino functions of glucosamine are protonated. These can then develop ionic interactions such as the fixation of
metallic anions, anionic dyes, and adhesion to negatively charged surfaces. These interactions also give to chitosan an excellent
film-forming property . At a basic pH, the amine functions are not in ionized form and can then form hydrogen bonds or covalent
amide or imine bonds with activated carboxylic acids and aldehydes, respectively. Concerning the semi-covalent approach, the amine
groups are positively charged for pH values < 6.5 and can form ionic bonds with the carboxylic acid groups . The alcohol functions
of glucosamine can mainly develop hydrogen bonds or covalent bonds. To develop each of these approaches, it was necessary to
take into account the acid-base constraints of glucosamine allowing the establishment of these specific bonds.
Also, these reactive groups offer to chitosan polymers many advantages and relevant properties (e.g. mucoadhesive properties,
absorption enhancer) ; they are easily processed into gels, films, membranes, nanofibers and nanofibrils, scaffolds, beads, sponge
forms, microparticles and nanoparticles [29,49]. In addition, chitosan possesses many more properties such as biocompatibility,
biodegradability, low toxicity and good antimicrobial and antioxidant activities leading to numerous applications . Table 2
summarizes the main properties of chitosan [28,52].
Table 2: Properties of chitosan
Physical and chemical properties Biological properties Linear amino polysaccharide
Reactive amino and hydroxyl groups Chelates many transitional metal ions Rigid D-glucosamine structure High hydrophilicity, crystallinity Deprotonated amino group
Form hydrogen bonds intermolecularly High viscosity
Soluble in water and organic solvents Soluble in dilute aqueous acidic solutions Polyelectrolytes (at acidic pH)
Biocompatibility Natural polymer Bioadhesivity Bioactivity Nontoxic Biodegradability Antimicrobial activity Antioxidant activity
Antiacid, antiulcer and antitumoral Blood anticoagulants
Entrapment, filtration, separation and adsorption
Film forming ability Hydrating agent
II.4. Chitosan solubility
Chitin is insoluble in many organic solvents due to the presence of acetyl group with a hydrophobic nature . Chitosan is the only
commercial water-soluble cationic biopolymer and it is soluble in dilute acidic solutions at pH values above 6.5 but insoluble in neutral
and alkaline aqueous solutions [43,55]. Table 3, shows some solutions used for the solubilization of chitosan.
Table 3: Some solutions used for the solubilization of chitosan
Acetic acid 1% 
Formic acid 0.2-100% 
Hydrochloric acid 1% 
Dilute nitric, succinic, lactic and malic acids 
Sulfuric and phosphoric acids 
Any neutral and alkaline pH aqueous solutions 
One of the most important properties of this polymer is the presence of the amine group with a pKa value of 6.5 in the carbonic chain.
With this termination, chitosan indeed has an acid-base behavior in solution, as shown in Figure 5. It is reported that the pKa value
increases with the ionic strength, thus widening the pH range in which chitosan is soluble .
Figure 5: Behavior of chitosan according to the pH of the solution
So, at pH <pKa the amino groups are positively charged which makes the chitosan a water-soluble cationic polyelectrolyte, and at
pH> pKa the biopolymer loses its charge and becomes insoluble . Indeed, at low pH, the chain is polycationic. Repulsive
electrostatic forces prevent the monomer associations which make chitosan soluble in solution. When pH increases, the chitosan
loses its positive charge, the balance between the forces of attraction and repulsion is then disturbed [31,58]. As discussed previously,
the solubility of chitosan in acidic medium is explained by the cationic character of its amine functions when they are protonated
providing sufficient electrostatic energy to break the numerous hydrogen bonds and considerably improve the hydration of the chains.
Therefore, the solubility of chitosan also depends on the distribution of the acetyl groups along the biopolymer chain and the DD
II.5. Chitosan stability
Chitosan is very sensitive to different experimental parameters that affect its stability; degree of deacetylation, molecular weight,
polymer concentration, type of acid and its concentration are parameters to take into account in the experiments .
- Temperature and pH effect
The main factors affecting the behavior of CS and its physical properties are pH and temperature. pH affect the polymer properties
due to the protonation and deprotonation of the amino groups . High temperature (>500 °K) may cause thermal degradation of
CS . Also, it has been reported that heat treatment can change the way the chains of the polymer react; this is attributed to the
influence of the ionic association of amine groups with alkanoic acids, such as formic, acetic, propionic, and butyric acid [61,62]. The
mechanism may involve an initial depolymerization followed by interchain cross-linking when the amount of heat assimilated is
sufficiently high .
- Humidity effect
Humidity is one of the factors affecting the behavior of chitosan. Studies show that exposing thin layers of chitosan to moist air causes
considerable swelling of the film. After heating and then cooling to the ambient temperature of these layers, a dramatic decrease in
thickness is recorded. These changes are not due to the oxidation or the thermal degradation of the films but it is suggested that the
heating irreversibly releases the trapped water .
Furthermore, studies on chitosan-based sensors show that, probably, in an airy medium, oxygen molecules are chemically absorbed
by chitosan (Equation 1). Once the film is subjected to a potential, the absorbed oxygen molecules react with the free electrons
forming ionic species such as O2- and O- (Equation 2-3), causing an increase in resistance to charge transfer until the oxygen
molecules are saturated. In the presence of water, the molecules in contact with chitosan react with O- to produce O2 and release
the electrons participating in the modification of the response of the sensor (Equation 4).
O2 O2 (absorbed) (1)
O2 (absorbed) + e- O2- (2)
O2- + e- 2O- (3)
CS-NH2 + 2O- + H2O CS-NH2 + O2 + H2O + 2e- (4)
In addition to reacting with O-, bonds can be formed between the oxygen of the water molecules and the hydrogen of the amino
groups of chitosan (Fig.6). These connections act as electrical bridges creating a surface tension facilitating the movement of the
Figure 6: Formation of hydrogen bridges by reaction between water molecules and CS amino groups 
II.6. Chemical modification of chitosan
Chitosan, by its hydroxyl functions and its primary amine, offers multiple possibilities of chemical functionalization, and allows easy
modifications including N substitution, O substitution and free radical graft copolymerization. These modifications have been proposed
in order to improve the intrinsic properties of CS (pore size, mechanical strength, chemical stability, hydrophilicity and also
biocompatibility) or to give new properties .
Chemical crosslinking is used to improve the stability and compatibility of chitosan and enhance its mechanical properties. Amine
and hydroxyl active groups on the biopolymer chain allow reactions with some chemical agents while undergoing structural changes.
These modifications are due to the creation of covalent bonds, -OH is more likely to participate in a nucleophilic reaction than amine
because of the stronger electronegativity of oxygen [66,67]. Several crosslinking agents have been established with chitosan (figure
7) including glutaraldehyde and glyoxal , N,N’-methylenebisacrylamide, 2-(chloromethyle) thiirane, ethylene glycol diglycidyl,
sulfuric acid , genipin , sodium tripolyphosphate , (3-glycidoxypropyl)trimethoxysilane , diisocyanates and
The chemical modification of the polymer makes it possible to modify its physical and chemical properties. Many modifications are
possible, in particular the grafting on the amine function of various chemical groups. The primary amine comprising a non-binding
doublet is a good nucleophile that will allow nucleophilic addition/elimination reactions on electrophilic carbons such as aldehydes,
ketones and carboxylic acid.
Many studies have examined the modification of chitosan. Chitosan has in particular been functionalized with benzaldehyde , 4-
nitrobenzoyl chloride and with glutaraldehyde , a compound having two aldehyde functions making it possible to create a covalent
bridge between chitosan and DNA fragments  or enzymes .
A widely used synthetic route for the biofunctionalization of chitosan is by forming an amide bond between the primary amine of
chitosan and the carboxylic acid function of the biomolecule to be fixed. This bond is difficult to implement and requires the prior
activation of the carboxylic acid function carried out by the 1-ethyl-3- (3-dimethylaminopropyl) carbodiimide and N-hydroxysuccinimide
(EDC/NHS) pair. This (non-detailed) activation mechanism consists of forming an intermediate ester between NHS and the carboxylic
Figure 7: Different types of crosslinking agents for chitosan
As presented in this part, chitosan is an abundant biosourced polymer, presenting functional groups that can be easily chemically
modified. It is soluble in aqueous solutions and it is well known to preserve the activity of biological molecules such as proteins .
Most of the template molecules are soluble in aqueous media, then these properties of chitosan are of interest for the preparation of
molecule template-polymer complex. The classical monomers used for MIP preparation, mainly vinylic and acrylic ones  are not
soluble in aqueous solution. This point could be deleterious for some template molecules such as peptides and proteins. Due to its
natural origin, chitosan is biodegradable, which is not the case of classical monomers that are not compatible with circular economy.
III. MIPs as recognition elements in electrochemical sensors
III.1. General principle of MIPs
The molecular imprinting technique illustrated in Figure 8 makes it possible to prepare polymers capable of selectively recognizing a
chosen molecule(s) commonly called target molecule(s) or template(s).
Figure 8: Schematic of molecularly imprinted polymers for two different templates.
step1: Pre-polymerization. Step 2: Polymerization and cross-linking. Step 3: Removal of template. Step4: Recognition
Molecularly imprinted polymers (MIPs) are artificial receptors prepared with a template, functional monomer and cross-linking agent.
The functional monomer interacts with the template forming a complex called “pre-polymerization complex”. In the presence of a
crosslinking agent, the complex is copolymerized in order to obtain a crosslinked polymer. After polymerization, the groups of
functional polymers are held in position to form a cast-type shell. The last step is then to extract the target molecules from the polymer.
Template molecules are removed by electrochemical or chemical extraction to disrupt the interactions between the template and the
monomers [77,78]. In essence, synthetic polymeric materials with specific recognition sites, complementary in shape, size and
functional groups to the template molecule are formed, through an interaction mechanism based on molecular recognition.
III.2. Response of MIPs electrochemical sensor
For a sensor to be effective, it must generate a measurable, and if possible quantifiable, physical signal during the interaction between
the target molecule and the MIPs (Figure 9).
Figure 9: Electrochemical response of MIPs sensor.
Selectivity, sensitivity, stability, reuse, response time, etc., are the main parameters in the design of sensors based on MIPs. These
parameters depend on both the properties of the MIP and its ability to interact with the analyte under the required conditions. These
parameters also depend on the sensitivity of the transducer and its ability to monitor the interaction process and transform it into a
measurable signal. It is therefore essential to choose not only a good combination between these two components but also the
electrochemical technique used.
Electrochemical measurements implemented in the case of sensors based on MIPs are very often conductimetry, potentiometry,
amperometry, voltammetry and impedancemetry. Conductometric sensors are based on the measurement of the change in
conductivity resulting from the recognition of the target molecules by the MIPs. A potentiometric sensor measures the potential
difference between the working electrode functionalized with MIPs and a reference electrode at zero current. The signal in
amperometric devices depends on the rate of charge transfer at the surface of the electrode. A voltammetric sensor measures the
variation of the intensity of the current in an interval of the applied potential. The impedance measurement is based on the
measurement of the variation in the charge transfer resistance of the MIPs. It is possible to link the results of the measurements to
the physical and chemical properties of the MIP-template interaction, and this by modeling the response by suitable equivalent
The choice of measurement technique is generally guided by the electrochemical properties of the target molecule. When the target
is electroactive, its presence in the medium to be analyzed will contribute to the modification of the intensity of the current; this change
could be followed by amperometry or voltammetry. If the target does not present any redox properties, the presence of the target will
cause a change in the MIP film, a behavior generally monitored by conductimetry or impedance.
III.3. Synthesis parameters of CS-MIPs
- Preparation of CS solution
The most commonly used acid for dissolving chitosan is acetic acid in aqueous solution, since the films of chitosan obtained with
acetic acid as solvent have properties to water . Acid solutions concentrated at high temperatures can depolymerize chitosan
, so, CS is generally prepared with diluted acid.
The choice of template during the synthesis of molecularly imprinted chitosan is of major importance, it must form the largest number
of specific well-defined interactions. Ideally, these interactions with the monomer should be strong to ensure better effectiveness. In
most studies, the molecule of interest is the template. However, for certain reasons such as rarity, high price, toxicity, difficulty in
handling, etc, the target molecule may be replaced by a molecule which is structurally and chemically analogous during synthesis.
For example, 2,4-dinitrotoluene (2,4-DNT) is used to form specific sites for the analysis to nitro explosives, as 2,4-DNT has a similar
structure with nitro explosives . However, one must be aware of the disadvantages of using a model with a structural similarity to
the analyte and ensure that the matrix does not interfere in the quantification .
The template to be used requires taking into account its structure and its functional groups, which make it possible to form bonds
with active groups of chitosan throughout the formation process of the template/biopolymer complex. Likewise, the size of the
template plays a role in the specificity of the cavities formed during imprinting. Indeed, for a high molecular weight template, there is
a risk that the small molecules might penetrate the cavities developing non-specific interactions . In addition, the larger templates
are less rigid and do not facilitate the creation of well-defined cavities. Also, large molecules such as peptides and proteins do not
easily penetrate the polymer network to occupy the cavities . The imprinting of small molecules, like pesticides and
pharmaceuticals, is well established in the synthesis of MIPs and considered routine; however the printing of much larger structures
remains a challenge.
Crosslinking is a key step in the synthesis of MIPs. The type of crosslinking agent and its proportion relative to the amount of functional
monomer are important in controlling the morphology of the polymer matrix and the selectivity of the cavities formed after the
extraction of the template, they allow:
ü Precise control of the imprinting of the template.
ü Complementary interactions with the target.
ü The mechanical stability of the imprints obtained and of the polymer.
ü The formation of a rigid matrix, resistant to high temperature and pressure conditions and inert towards acids and bases
For a MIPs synthesized in a polar solvent, it is important to choose a hydrophilic crosslinker to facilitate contact with the surface of
the polymer. Also, the use of MIPs crosslinked with a hydrophobic agent remains unstable in aqueous media.
To crosslink the chitosan used in sensors based on MIPs, two methods are used; either the crosslinking agent is mixed with the
template/polymer complex before deposition on the working electrode surface; in this case the crosslinking agent/functional monomer
ratio is very important . The second method is based on the deposition of the template/polymer complex on the electrode and
then impregnating the modified electrode in the cross-linker solution. Here, the concentration of the crosslinking solution and contact
time define the properties of the prepared MIPs .
III.4. Principle of the electrodeposition of chitosan
The ability to create devices like sensors and biosensors requires easy methods to precisely control surfaces. A variety of techniques
can be used to produce the desired structures. The integration of a chitosan-MIP with the transducer area is a crucial step in the
fabrication of the sensor. The biopolymer material must adhere well to this surface without dispersing or detaching under any
conditions. The properties of chitosan have been used to make membranes, thin films and three-dimensional structures by various
methods such as drop coating , microcontact, complexation with anionic polyelectrolytes .
The pH-sensitive solubility and properties of chitosan have also been used to make membranes, thin films and three-dimensional
structures. Chitosan changes from a soluble state in acid solution to a precipitated hydrogel state when the pH of the solution
increases. CS can be easily poured, producing membranes and films which can be converted into insoluble networks by
neutralization. The cast chitosan membranes/films can be made insoluble over the entire pH range by covalently crosslinking the
chitosan chains by amide and imine interactions.
Electroaddressing is used for the deposition of chitosan in the field of electrochemical sensors; it consists in applying a cathodic
voltage to the surface of an electrode. Electrodeposition has the advantage of being a simple, fast and low cost technique. It is an in
situ process that combines precipitation and immobilization. The electrodeposition of chitosan makes it possible to obtain very porous
films in a spatially selective and modeled manner . This technique has been used successfully to deposit chitosan films on
conductive electrodes [90,91]. More specifically, the chitosan can be electrodeposited on the surface of a cathode by the mechanism
illustrated in the figure 10.
Figure 10: chitosan electrodeposition mechanism
Local pH is increased, close to the cathode surface, due to the electrochemical reduction of water, according to the following reaction:
2 H2O + 2 e- H2+ 2 OH- (5)
The pH varies as a function of the relative rates of hydroxyl ion generation and hydroxyl ion diffusion from the interfacial region. The
hydroxyl ions generated are adjusted by the voltage applied to the surface of the electrode. In the presence of the slightly acidic
solution of chitosan, a pH gradient is established in the vicinity of the surface of the cathode. In localized regions with a high pH above
6.5 the chitosan is deprotonated and becomes insoluble. Depending on the conditions, this causes precipitation of the polymer and
the formation of a homogeneous membrane on the surface of the cathode . A pH gradient near the electrode allows the
precipitation of chitosan during the application of the potential, pH 5 being considered as the optimal pH of the electrodeposition.
III.5. Chitosan electrodeposition techniques
The two most commonly used techniques for the electrodeposition of chitosan are cyclic voltammetry (CV) and chronoamperometry
a- Electrodeposition by CV
Figure 11 shows the electrodeposition voltammograms of chitosan on gold macroelectrodes at pH 5 . A CV of the chitosan solution
prepared in 0.1M acetic acid was carried out with a potential varying between -1.5 V and 0.5 V at a scan rate of 80 mV/s. There is a
cathodic peak characterizing the electrodeposition of the polymer. The peak intensity gradually decreases according to the scan
number, a sign of precipitation of the polymer on the surface of the electrode. Beyond a few scans, the intensity of the peak does not
vary, which makes it possible to fix the number of scans. This test shows that a constant voltage between -1.3V and -1.1V is optimal
for chronoamperometry deposition, preventing an excessive yield of hydrogen gas affecting the deposition and adherence of the
Figure 11: CV of electrodeposition of chitosan on gold microelectrode at pH 5 and a scan rate of 80 mV/s.
b- Electrodeposition by CA
Figure 12 shows the curves obtained during the electrodeposition of chitosan by CA on gold macroelectrodes at pH 5 and an applied
voltage of -1.1V . After a decrease in the negative current, a plateau is observed, a sign that the reaction by diffusion of H+ at the
surface of the electrode has been limited. The formation of this plateau indicates the effective deposition of the polymer, which makes
it possible to optimize the time of the electrodeposition.
-1,5 -1,0 -0,5 0,0 0,5
-0,10 -0,08 -0,06 -0,04 -0,02 0,00 0,02
Potential (V) Scan 2 Scan 7 Scan 16
Figure 12: CA of electrodeposition of chitosan on gold microelectrode area at pH 5 and potential of -1.1 V.
Chitosan can be deposited in a controllable manner. The thickness of the electrodeposited chitosan film can vary as a function of the
pH of the solution and electrochemical deposition conditions such as the time and the potential applied for the CA, the potential
interval, the number of cycles and the scan rate for CV.
III.6. Removal of the template
The last step in the MIP process is to extract the target molecules from the biopolymer. Extraction of the imprinted model is an
important step in the manufacture of MIPs, and for this purpose, numerous protocols have been established. The choice of procedure
must take into account the efficiency of the extraction while maintaining the structure without causing any degradation of the matrix
(by solvent, temperature, etc.).
Templates are removed from the MIPs by electrochemical or chemical extraction, allowing disturbance of the interactions of the
prepolymerization complex. Indeed, non-covalent interactions such as hydrogen interactions can be "broken" by washing with
solutions of different pH .
However, this step does not lead to the complete extraction of the template from the polymer; more than 1% of the template used
during the synthesis of MIPs remains bonded to the polymer even after intensive washing . As a result, not only is there a decrease
in active sites, but also large dosing errors can then occur due to the slow release of the remaining molecules when using MIPs .
III.7. MIPs electrochemical sensors based on chitosan
Due to its macromolecular structure (carrying an excess of amine and hydroxyl groups), its physico-chemical and biological
properties, the use of chitosan in molecularly imprinted polymers has attracted considerable attention. The fact that chitosan has an
affinity for various compounds and the possibility of complexing the template or of undergoing chemical modifications by means of
different approaches (non-covalent, semi-covalent, covalent) can be easily exploited for the construction of MIPs.
Due to its relevant structural benefits of being easily transformed into gels, films, membranes, nanofibers and nanofibrils, scaffolds,
beads, sponge forms, microparticles and nanoparticles, molecular imprinted chitosan is widely used in various applications such as
solid-phase extraction , selective separation of proteins , therapeutic studies [97,98], sensors , etc. The properties of MIPs
such as specificity and high stability, compatibility with microfabrication technology and low cost make them promising alternatives to
the antibodies and other natural receptors usually used .
Several sensors have been developed using MIPs as mentioned above such as electrochemical, colorimetric, fluorescent sensors,
etc. Given the predominance of electrochemical sensors on the market due to their simplicity, sensitivity, ease of implementation and
generally low measurement costs, this review will focus on the development of electrochemical sensors based on molecularly
imprinted chitosan (CS -MIPs). Many successful examples of the development of electrochemical sensors based on chitosan-MIPs
for different templates such as metabolites (dopamine, L-dopa, glucose, urea), pesticides (trichlorphon, glyphosate), medications
(clenbuterol, epinephrine) and phenolic compounds (p-nitrophenol, 2,4,6 tribromophenol, bisphenol A, catechol), are reported in
Table 4. The detected molecules generally present a molecular weight between 100 and 200 g/mol. The common characteristics of
these molecules is that they present hydroxyl and amine groups in their structure. Ion-imprinted sensors based on chitosan have also
been developed for the detection of chromium (VI), cadmium and copper, due to the ion coordination with hydroxyl and amine groups
in the glucosamine units.
Electrochemical sensors combined with molecularly imprinted chitosan showed good performance. The proposed sensors exhibited
a good linear response towards several targets with a low detection limit, good selectivity, reproducibility, stability and reusability.
The preparation procedures presented are relatively simple, convenient and provided rapid and economical methods [101–103].
Pulse Differential Voltammetry (DPV) is the most used electrochemical technique in MIP-based sensors. The results obtained show
low detection limits, reaching 10-12 M for the target molecule urea, and a slightly higher LOD in the case of dopamine (10-11M)
. LOD is in the order of 10-7 to 10-9M with phenolic compounds [56,78,101,105]. The majority of these sensors can be reused up
to 9 or 10 times [78,102–104,106], and others less for example 5 times with the target molecules 2,4,6-tribromophenol  and
copper ions .
CA and CV are used in several studies. The detection limits are between 10-5 and 10-9 M [24,25,108,109]. Some sensors have been
regenerated 9 times [108,110], and others less, for example 7 times in the case of bisphenol A , 3 times with catechol [24,25].
The lowest detection limit recorded is 10-21M. The technique used was Square wave voltammetry (SWV) for the detection of bisphenol
A . Another, of 5.9x10-18 M, has been described using electrochemical impedance spectroscopy, for the detection of glyphosate
A MIP sensor, using CV in the presence of [Fe(CN)6]3-/4- is presented by Y.-P. Chen et al (Fig.13). The electrochemical sensor was
474constructed based on chitosan molecularly imprinted films, which were prepared by electrodeposition of chitosan in the presence of
475template (urea) using CA at -1.1 V for 3 min on the Au disk electrode for the determination of urea. In order to elute the template
476molecules, the (urea+CS)/Au was placed in KCl solution. The sensor was characterized using CV in [Fe(CN)6]3-/4- solution to
477determine the urea indirectly in the range from 10-8 to 4×10-5 M with a detection limit of 5×10-9 M. The sensor offers great potential
478for clinical diagnosis applications .
Figure 13: Schematic illustration of a MIP electrochemical sensor fabrication for the detection of urea.
III.8. Nanomaterial doped-CS
The electrochemical performance of electrodeposited CS film on the surface of the working electrode is limited by poor electrical
conductivity. Indeed, due to the high degree of crystallinity that the polymer has, conductivity is low, which hinders the redox process
. To overcome this problem, the use of nanomaterials with electroactive functionality is of great interest in the development of
electrochemical sensors based on molecularly imprinted chitosan, due to the fact that nanomaterials can improve the electron transfer
between the electrode surface and the solution, so improving the sensitivity of chitosan-based sensing material. Nanomaterials such
as gold nanoparticles , silver nanoparticles , CuCo2O4 carbon nanocomposites , ZnO nanoparticles , acetylene
black , carbon nanotubes , Graphene , multiwalled carbon nanotubes  have been applied to modify electrode
because of their excellent electrocatalytic activity.
An example of a chitosan-graphene based sensor is that by S. Wu et al  in which the fabrication process sensor is based on the
electrodeposition of the chitosan-graphene nanocomposite and the template (Cr (VI)) on the Au disk electrode, for the determination
of Cr (VI). The different steps for the fabrication of the MIP-based sensor are presented in Figure 14. Electrodeposition was performed
using CA at −1.2 V for 180s. Glutaraldehyde was used to crosslink the chitosan-graphene-Cr (VI) film. The obtained imprinted
electrode was successively rinsed with acetone/water to remove the template. The detection was performed using DPV in a linear
range from 10−9 to 10−5 mol/L, with a low detection limit of 6.4×10−10 mol/L. The proposed sensor was successfully applied to the
detection of Cr(VI) ions in tap water and river water.
500 501 502
Figure 14: Schematic representation of the fabrication process of chitosan-graphene MIP sensor for Cr (VI) detection.
507In the work of A. Fatoni et al (Fig.15), a MIP sensor was prepared by dropping onto the gold rod electrode the mixture of CS,
508acrylamide, N,N’-methylenebisacrylamide, graphene, ferrocene and microalbumin as template. The template was removed from the
509modified electrode by soaking in acetic acid-sodium dodecylsulfate solution. The specific imprinted surface was used to detect
510microalbumin from 1.5×10-9 to 1.5×10-7 M via a redox mediator (ferrocene), entrapped in the cryogel, using differential pulse
511voltammetry (DPV). The limit of detection was 7.7×1013 M and the excellent performance of the biosensor was confirmed by analyzing
512microalbumin in urine samples .
Figure 15: Schematic representation of the fabrication process of MIP sensor chitosan grafted polyacrylamide MIP cryogel
516with graphene and entrapped ferrocene for the detection of microalbumin.
Table 4: Electrochemical sensors based on CS-MIPs.
Cross-linking Extraction of template
Samples Linear range Limit of detection
/ CA in KCl and
Blood serum 10-9 M – 8.10-8 M 10-7 M – 10-4 M
10-11 M / 
/ KCl and ethanol PBS solution 0,51.10-6 M – 1,95.10-3 M
0,16. 10-6 M / 
/ KCl and ethanol PBS solution 0,12.10-9 M – 1,52.10-4M
0,039. 10-9 M / 
/ CA in KCl and
Blood serum 4.10-7 M – 10-4 M 0,012. 10-6 M / 
/ KCl solution Blood serum 5.10-12 M – 4.10-10 M 5.10-10 M – 7.10-8 M
10-12 M 10 
/ Acetic acid and
Urine samples 1,5.10-9 M – 1,5.10-7 M
7,7.10-13 M 9 
P-nitrophenol CS+PTMS+AuN Ps+T/
/ CV in acetate buffer Acetate buffer solutions
3.10-8 M – 5,5.10-4 M
5.10-9 M 10 
Sulfuric acid Sulfuric acid Clean water 10-7 M – 10-3 M 1,32.10-8 M 5 
Bisphenol A CS+AB+T/
Sulfuric acid Methanol and acetic acid
Drinking water 5.10-9 M – 2.10-7 M 5.10-7 M – 10-5 M
2. 10-9 M / 
CA in KCl Tea sample 5.10-7 M – 10-5 M 10-7 M / 
ethylenediaminetetr aacetic acid
Tap and river water
10-9 M – 10-5 M 6,4.10-10 M 9 
copper ions CS+Gr+T/
ethylenediaminetetr aacetic acid
tap and river water
5.10-7 M – 10-4 M 0,15.10-6 M 5 
cadmium ions CS+AuNPs+Gr+
drinking water and milk samples
10-7 M – 9.10-7 M 1,62.10-4 M 10 
/ KCl solution Blood serum and
10-8 M – 4.10-5 M 5.10-9 M 9 
CV/Modified WGE/B-R Buffer
Sulfuric acid CA in acetic acid, phosphoric acid and boric acid solution
Pork liver 3.10-7 M – 5.10-5 M 0,01.10-6 M 5 
Sulfuric acid Sulfuric acid Plastic samples 8.10-8 M – 10-5 M 60.10-9 M 7 
Catechol CS+AuNPs+MW CNT+T/
KCl solution wine sample 7,5.10-5 M – 10-3 M 3,7.10-5 M 3 
/ KCl solution wine sample 5.10-5 M – 7,5.10-5 M
6,9.10-7 M 3 
bisphenol A CS+T/
Ethanol and acetic acid
drinking water 10-3 M – 10-21 M 0,67.10-21 M 10 
Bisphenol A CS+Gr+T/
Sulfuric acid CV in HCl Drinking water and canned beverages
8.10-9 M – 10-6 M 10-6 M – 20.10-6 M
6.10-9 M 10 
/ water elution KOH solution 10-5 M – 20.10-5 M 2.10-6 M / 
/ KCl and ethanol PBS solution 0,12. 10-9 M – 152. 10-6 M
0.039.10-9 M / 
Epinephrine CS+PIL+MWCN T+T/
/ phosphate buffer
phosphate buffer solution
0,2. 10-6 M – 0,67.10-3 M
60.10-9 M 9 
Sulfuric acid Ethanol and acetic acid
River water 1,83. 10-15 M – 3.10-10 M
5,9. 10-18 M 2 
DPV: Pulse Differential Voltammetry CA: Chronoamperometry
SWV: Square wave voltammetry CV: Cyclic Voltammetry
LSV: Linear Sweep Voltammetry EIS: Electrochemical Impedance Spectroscopy Au: Gold electrode
GCE: Glass Carbon Electrode
IE1: Integrated electrode CuCo2O4@carbon nanocoposites/Three-dimensional kenaf stem-derived marcoporous carbon IE2: Integrated electrode ZnO@carbon nanocoposites/Three-dimensional kenaf stem-derived marcoporous carbon Modified WGE: electrode Nano-silver/Quercetin/Working graphite
ABPE: Acetylene Black Paste Electrode BDD: Bored-Doped Diamond electrode NiOE: Nickel Oxide Electrode
PBS: Phosphate Buffer Solution B-R Buffer: Britton-Robinson Buffer HAc-NaAc: Acetic acid-Sodium Acetate T: Template
Gr: Graphene QDs: Quantum Dots AM: Acrylamide
PTMS: Phenyltrimethoxysilane AuNPs: Gold Nanoparticles AB: Acetylene Black
MWCNT: Multiwalled carbon nanotubes